TechBrief: Long-Life Concrete Pavements: Best Practices and Directions From the States
- Practices and Directions of State Department of Transportation
The International Conference on Long-Life Concrete Pavements was organized in October 2006 as a part of technology transfer activities for the Concrete Pavement Technology Program (CPTP), which operates within the Federal Highway Administration (FHWA) (Tayabji and Lim 2006). The conference objective was to provide a forum to address various aspects of concrete pavement design, construction, and materials technologies that result in long life for concrete pavements. Several State departments of transportation (DOTs) participated in the conference and presented information related to their current practices and future directions for achieving long-life concrete pavements. This TechBrief summarizes the long-life concrete pavement practices presented by the Illinois, Minnesota, Texas, and Washington State DOTs, practices that are representative of directions implemented by States that have strong concrete pavement construction programs.
In the past, concrete pavements were routinely designed and constructed to provide low-maintenance service lives of 20 to 25 years. In fact, the majority of pavements in the interstate and primary systems in the United States were designed on the basis of a 20- to 25-year initial service life. More recently, there has been a movement toward construction of pavements with a longer initial service life-40 or more years, particularly in high-volume, urban corridors where traffic disruptions and user delays can be especially acute because of frequent or extended lane closures. The use of long-life pavement strategies has proven to be a cost-effective tool for minimizing maintenance costs and reducing user delays for many highway agencies in the United States. As an example, the California Department of Transportation (Caltrans) requires use of a 40-year service life for designing pavements along a highway corridor where the 20-year projected average annual daily traffic equals or exceeds 150,000 vehicles or average annual daily truck traffic equals or exceeds 15,000 trucks (Caltrans 2006).
Long-life concrete pavements (LLCPs) have been quite attainable for a long time in the United States, as evidenced by the number of very old pavements that remain in service; however, recent advances in design, construction, and concrete materials technology give us the knowledge and technology needed to consistently achieve what we know to be attainable.
A useful definition of long-life concrete pavement in the United States is summarized as follows (Tayabji and Lim 2006):
- Original concrete service life is 40+ years.
- Pavement will not exhibit premature construction and materials-related distress.
- Pavement will have reduced potential for cracking, faulting, and spalling.
- Pavement will maintain desirable ride and surface texture characteristics with minimal intervention activities, if warranted, for ride and texture, joint resealing, and minor repairs.
The quest for long-life concrete pavements necessitates a much better understanding of design and construction factors that affect both short-term and long-term concrete pavement performance. Essentially, this requires that there be a better understanding of how concrete pavements deteriorate or fail. Concrete pavements deteriorate over a period of time as a result of distresses that develop due to a combination of traffic and environmental loading. Typical distresses that can develop include the following:
- Cracking-Typically transverse cracking occurs, but longitudinal, random, and corner cracking may also develop due to poor design and construction practices. Cracking is typically referred to as a stress-based distress.
- Joint faulting-Joint faulting may develop with or without outward signs of pumping. Faulting is typically referred to as a deflection-based response. Joint faulting is significantly affected by the type of load transfer provided at transverse joints.
- Spalling-Spalling may develop along joints or cracks and may be caused by poor joint-sawing practices, incompressible materials in joints or cracks, winter snow removal operations, or poor-quality concrete.
- Materials-related distress-The more significant materials- related distresses may include alkali-silica reactivity (ASR) and D-cracking in freezing environments.
- Roughness-The lack of pavement smoothness, or roughness, is affected by the development of various distresses in the concrete pavement, as listed in items 1 through 4 above. The effect of each distress type is additive and results in pavement roughness over a period of time. Some pavement roughness is also built in during construction. Initial pavement smoothness is needed in order that the pavement does not become prematurely rough. Construction specifications typically utilize incentives and disincentives to control new pavement smoothness.
- Texture loss-Although not conventionally considered a distress, texture loss is a significant distress for pavements in high-volume, high-speed applications.
It is realized that it would be impossible or impractical to design and construct concrete pavements that exhibit very little or no distress. Distress development over the pavement's service life is expected. However, the rate of distress development is managed by incorporating sound designs, durable paving materials, and quality construction practices. Generally recognized threshold values in the United States for distresses at the end of the pavement's service life are listed in Table 1 for jointed plain concrete pavements (JPCPs) and continuously reinforced concrete pavements (CRCPs).
|Cracked slabs, % of total slabs (JPCP)||10 to 15|
|Faulting, mm (in.) (JPCP)||6 to 7 (0.25)|
|Smoothness (IRI), m/km (in./mi) (JPCP and CRCP)||2.5 to 3.0 (150 to 180)|
|Spalling (length, severity) (JPCP and CRCP)||Minimal|
|Materials-related distress (JPCP and CRCP)||None|
|Punchouts, no. per km (mi) (CRCP)||10 to 12 (16 to 20)|
JPCP = jointed plain concrete pavement, CRCP = continuously reinforced concrete pavement, IRI = International Roughness Index
Typical pavement performance trends are illustrated in Figure 1. When the pavement service-ability has reached the threshold level, the pavement no longer efficiently or safely serves the driving public. This corresponds to the point in time at which one or more of the distress threshold values listed in Table 1 is reached. In the past, the threshold levels were expected to be reached at about 20 to 25 years. The threshold would be reached earlier if the pavement incorporated design or construction deficiencies. For long-life pavements, the threshold is expected to be reached at 40+ years.
Figure 1. Pavement performance trends.
The above requirements can be met only through sound pavement design, use of durable materials, ensured quality during construction, and timely maintenance. Design and construction of a successful concrete pavement require attention to many details, and most require little additional effort to be performed correctly.
Practices and Directions of State Departments of Transportation
During the late 1990s, the Illinois DOT (IDOT) began investigating concepts in the design and construction of extended-life concrete pavements. IDOT carried out the following activities (Winkelman 2006):
- Cooperative research with the University of Illinois-Accelerated testing was performed to determine the optimal structural design features for CRCP.
- Identification of long-life design and construction features-Structural design features, concrete materials requirements, and construction processes were refined.
- Construction projects-To demonstrate the feasibility of the construction of long-life pavement, several projects were constructed across the State.
Subsequently, IDOT's concrete pavement construction specifications were changed to incorporate rigorous concrete materials requirements to prevent freeze-thaw and ASR-related damage and to tighten construction tolerances. Details of the changes are summarized in Table 2.
The changes in the specifications were successfully incorporated in five demonstration projects, and the performance of the pavements has been excellent to date. IDOT is pursuing additional extended-life concrete pavement projects and will be incorporating more of the extended-life features into the current standard design procedure.
|Item||Long-Life Pavement Specification Change|
JPCP = jointed plain concrete pavement, IDOT = Illinois Department of Transportation, CRCP = continuously reinforced concrete pavement, AASHTO = American Association of State Highway and Transportation Officials
The Minnesota DOT (MnDOT) has adopted LLCPs as the standard design for high-volume, urban highways since 2000. The current design features and construction specifications associated with the LLCP are provided in Table 3 (Burnham et al. 2006).
Although LLCP has been successfully implemented in a number of projects within Minnesota, MnDOT continues to investigate concerns related to the expected service life of LLCP. MnDOT's concerns include concrete durability and construction-related issues. Current materials specifications used in the design of LLCP rely on accelerated laboratory testing. However, the laboratory performance may significantly differ from actual long-term performance in the field. There is concern whether the permeability and air content systems in the LLCP will be able to provide the necessary level of durability for the entire design period under the State's extreme climate conditions.
MnDOT has also experienced some construction problems from the use of new materials. Most LLCP projects include supplementary cementitious material (SCM) to meet the concrete mixture requirements. Many contractors who were not familiar with the LLCP concrete mixtures containing SCM have complained of difficulties in handling these mixtures. In this regard, training of the engineers and contractors will be critical for continuous success of LLCP in the future.
|Alkali-silica reactivity (ASR)||
MnDOT = Minnesota Department of Transportation, ASTM = American Society for Testing and Materials, GGBFS = ground granulated blast furnace slag, w/cm = water to cementitious material ratio
The Texas DOT (TxDOT) uses CRCP as the primary LLCP. Over the years, TxDOT has observed that the primary distresses in CRCP are punchouts, wide cracks, spalling, and construction joint failures. Based on the results of many investigations, TxDOT identified the primary causes of these distresses and modified its design and construction practices to provide longer lasting pavements, as shown in Table 4 (Won et al. 2006). The current practices followed by TxDOT to achieve LLCP are summarized in Table 5 (Won et al. 2006).
|Construction joint failure||
PCC = portland concrete cement; CTE = co-efficient of thermal expansion
|Longitudinal steel design|
AASHTO = American Association of State Highway and Transportation Officials, CTE = co-efficient of thermal expansion
About 38 percent of concrete pavements in Washington State were over 35 years old as of 2006. These pavements have lasted longer than their original 20-year design life with little or no maintenance or rehabilitation. Three primary distress types have been observed on the concrete pavements in the State: joint faulting due to lack of dowel bars and to poor conditions in underlying layers; longitudinal cracking that is believed to have occurred during the early years; surface wear due to studded tires.
Based on experience over the last 40 years and studies related to pavement performance, Washington State DOT (WSDOT) has modified its materials, design, and construction practices to achieve LLCP, as summarized in Table 6 (Muench et al. 2006).
|Studded tire mitigation|
PCC = portland cement concrete, HMA = hot-mix asphalt, AASHTO = American Association of State Highway and Transportation Officials, ASTM = American Society for Testing and Materials, HOV = high occupancy vehicle, GGBFS = ground granulated blast furnace slag
The extended-life design and construction practices have been successfully implemented in a number of concrete pavement projects in Washington State. WSDOT continues to study concrete- and dowel-bar-related issues to ensure that these materials will provide the required long-term durability. The durability of the concrete surface in the presence of studded tires, tire-pavement noise, and need for accelerated construction in the Seattle area are expected to drive future developments in LLCPs.
Presentations at the International Conference on LLCP indicated that many U.S. highway agencies have begun to implement strategies to achieve LLCPs that will provide a low-maintenance service life of 40 or more years. As reported in this TechBrief, the effort by most of these agencies involves refining design and construction practices and requiring improved construction quality control. The current directions indicate that no "out of the box" technologies are necessary to achieve LLCPs. As stated in the introduction to this TechBrief, long-life concrete pavements have been attainable for quite a long time in the United States, as evidenced by the number of very old pavements that remain in service. However, recent advances in design, construction, and concrete materials technology give us the knowledge and technology needed to consistently achieve what we already know to be attainable.
Burnham, T., B. Izevbekhai, and P. R. Rangaraju. 2006. "The Evolution of High-Performance Concrete Pavement Design in Minnesota," Proceedings, International Conference on Long-Life Concrete Pavements, pp. 135-151, held in Chicago, IL, October 25-27, 2006. Federal Highway Administration, Washington, DC.
Caltrans. 2006. Highway Design Manual, Chapter 610-Pavement Engineering Considerations. September 1, 2006. California Department of Transportation, Sacramento.
Muench, S., L. Pierce, J. Uhlmeyer, and K. Anderson. 2006. "The Evolution of Long-Life Concrete Pavements in Washington State," Proceedings: International Conference on Long-Life Concrete Pavements, pp. 19-35, held in Chicago, IL, October 25-27, 2006. Federal Highway Administration, Washington, DC.
Tayabji, S., and S. Lim (eds.). 2006. Proceedings, International Conference on Long-Life Concrete Pavements, held in Chicago, IL, October 25-27, 2006, Federal Highway Administration, Washington, DC.
Winkelman, T. J. 2006. "Design and Construction of Extended Life Concrete Pavements in Illinois," Proceedings, International Conference on Long-Life Concrete Pavements, pp. 3-18, held in Chicago, IL, October 25-27, 2006. Federal Highway Administration, Washington, DC.
Won, M., D. Kim, Y. Cho, and C. Medina-Chavez. 2006. "Long-Term Performance of Continuously Reinforced Concrete Pavement in Texas," Proceedings of the International Conference on Long-Life Concrete Pavements, pp. 171-180, held in Chicago, IL, October 25-27, 2006. Federal Highway Administration, Washington, DC.
Contact-For information about the Federal Highway Administration's (FHWA's) activities related to long-life concrete pavement, contact the following:
Federal Highway Administration
Office of Pavement Technology
CPTP Implementation Team
Research-This Techbrief was developed by Shiraz Tayabji, Ph.D., P.E., and Seungwook Lim, Ph.D., P.E., CTLGroup, as part of FHWA's CPTP Task 65 product implementation activity. This publication is based on papers presented at the International Conference on Long-Life Concrete Pavements held in Chicago, Illinois, October 2006, organized as part of FHWA's CPTP Task 65 product implementation activity.
Distribution-This TechBrief is being distributed according to a standard distribution. Direct distribution is being made to the Resource Centers and Divisions.
Availability-This document is based on papers presented at the International Conference on Long-Life Concrete Pavements. For information on the availability of the conference proceedings, please refer to the contact information above.
Key Words-Concrete, concrete pavement, pavement construction, pavement design, pavement performance.
Notice-This TechBrief is disseminated under the sponsorship of the U.S. Department of Transportation in the interest of information exchange. The TechBrief does not establish policies or regulations, nor does it imply FHWA endorsement of the conclusions or recommendations. The U.S. Government assumes no liability for the contents or their use.
Quality Assurance Statement-FHWA provides high-quality information to serve Government, industry, and the public in a manner that promotes public understanding. Standards and policies are used to ensure and maximize the quality, objectivity, utility, and integrity of its information. FHWA periodically reviews quality issues and adjusts its programs and processes to ensure continuous quality improvement.
The Concrete Pavement Technology Program (CPTP) is an integrated, national effort to improve the long-term performance and cost-effectiveness of concrete pavements. Managed by the Federal Highway Administration through partnerships with State highway agencies, industry, and academia, CPTP's primary goals are to reduce congestion, improve safety, lower costs, improve performance, and foster innovation. The program was designed to produce user-friendly software, procedures, methods, guidelines, and other tools for use in materials selection, mixture proportioning, and the design, construction, and rehabilitation of concrete pavements.